#------------------------------------------------------------------------------
#$Date: 2016-02-05 01:36:39 +0200 (Fri, 05 Feb 2016) $
#$Revision: 176048 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/74/7037406.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7037406
loop_
_publ_author_name
'Wang, Yanyan'
'Han, Tian'
'Ding, You-Song'
'Zheng, Zhiping'
'Zheng, Yan-Zhen'
_publ_section_title
;
 Sodalite-like rare-earth carbonates: a study of structural transformation
 and diluted magnetism.
;
_journal_issue                   3
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1103
_journal_page_last               1110
_journal_paper_doi               10.1039/c5dt03314d
_journal_volume                  45
_journal_year                    2016
_chemical_formula_sum            'C H6 Cl O9 Y3'
_chemical_formula_weight         464.24
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           229
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-10-07 deposited with the CCDC.
2015-11-23 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   12.665(9)
_cell_length_b                   12.665(9)
_cell_length_c                   12.665(9)
_cell_measurement_temperature    296(2)
_cell_volume                     2031(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker Apex \/cò DUO'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0526
_diffrn_reflns_av_sigmaI/netI    0.0314
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            2253
_diffrn_reflns_theta_full        26.90
_diffrn_reflns_theta_max         26.90
_diffrn_reflns_theta_min         2.27
_exptl_absorpt_coefficient_mu    17.281
_exptl_absorpt_correction_T_max  0.4787
_exptl_absorpt_correction_T_min  0.4787
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.035
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1744
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.923
_refine_diff_density_min         -1.350
_refine_diff_density_rms         0.317
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.117
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     21
_refine_ls_number_reflns         251
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      1.108
_refine_ls_R_factor_all          0.0884
_refine_ls_R_factor_gt           0.0701
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1047P)²+92.6412P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1868
_refine_ls_wR_factor_ref         0.2061
_reflns_number_gt                197
_reflns_number_total             251
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5dt03314d2.cif
_cod_data_source_block           3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Cubic' changed to 'cubic' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7037404--7037407.cif.
;
_cod_original_cell_volume        2032(2)
_cod_original_sg_symbol_H-M      Im-3m
_cod_database_code               7037406
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'x+1/2, z+1/2, -y+1/2'
'-x+1/2, z+1/2, y+1/2'
'-x+1/2, -z+1/2, -y+1/2'
'x+1/2, -z+1/2, y+1/2'
'z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, x+1/2'
'-z+1/2, -y+1/2, -x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y, -x, z'
'y, x, z'
'-y, x, -z'
'y, -x, -z'
'-x, -z, y'
'x, -z, -y'
'x, z, y'
'-x, z, -y'
'-z, -y, x'
'-z, y, -x'
'z, -y, -x'
'z, y, x'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z+1/2, x+1/2, y+1/2'
'z+1/2, x+1/2, -y+1/2'
'z+1/2, -x+1/2, y+1/2'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z+1/2, x+1/2'
'-y+1/2, z+1/2, x+1/2'
'y+1/2, z+1/2, -x+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-x+1/2, -z+1/2, y+1/2'
'x+1/2, -z+1/2, -y+1/2'
'x+1/2, z+1/2, y+1/2'
'-x+1/2, z+1/2, -y+1/2'
'-z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, -x+1/2'
'z+1/2, y+1/2, x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cl1 Cl 0.292(3) 0.5000 0.5000 0.305(15) Uani 0.67 8 d SPDU
O1 O 0.1768(10) 0.3232(10) 0.2500 0.036(5) Uani 0.50 2 d SP
C1 C 0.2500 0.2500 0.2500 0.019(6) Uani 1 12 d S
O2 O 0.1068(8) 0.5000 0.3320(8) 0.039(3) Uani 1 2 d S
H2A H 0.1675 0.5000 0.3800 0.047 Uiso 1 2 calc SR
Y1 Y 0.15390(13) 0.5000 0.15390(13) 0.0327(8) Uani 1 4 d SD
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 O1 C1 60.000(1) 77 .
O1 O1 O1 120.000(2) 77 81
C1 O1 O1 60.000(1) . 81
O1 O1 Y1 75.2(3) 77 .
C1 O1 Y1 134.2(3) . .
O1 O1 Y1 162.3(2) 81 .
O1 O1 Y1 162.3(2) 77 81
C1 O1 Y1 134.2(3) . 81
O1 O1 Y1 75.2(3) 81 81
Y1 O1 Y1 91.6(6) . 81
O1 C1 O1 60.0 9 77
O1 C1 O1 60.000(1) 9 73
O1 C1 O1 120.000(1) 77 73
O1 C1 O1 120.000(1) 9 .
O1 C1 O1 60.000(1) 77 .
O1 C1 O1 180.000(3) 73 .
O1 C1 O1 120.000(1) 9 5
O1 C1 O1 180.0(8) 77 5
O1 C1 O1 60.000(1) 73 5
O1 C1 O1 120.000(1) . 5
O1 C1 O1 180.000(3) 9 81
O1 C1 O1 120.000(1) 77 81
O1 C1 O1 120.000(1) 73 81
O1 C1 O1 60.000(2) . 81
O1 C1 O1 60.000(2) 5 81
Y1 O2 Y1 102.6(3) . 81
Y1 O2 Y1 102.6(3) . 34
Y1 O2 Y1 110.0(4) 81 34
O2 Y1 O2 119.6(5) 22_565 .
O2 Y1 O2 73.6(4) 22_565 77
O2 Y1 O2 144.21(15) . 77
O2 Y1 O2 144.21(15) 22_565 38
O2 Y1 O2 73.6(4) . 38
O2 Y1 O2 78.4(5) 77 38
O2 Y1 O2 73.6(4) 22_565 78_554
O2 Y1 O2 144.21(15) . 78_554
O2 Y1 O2 69.3(4) 77 78_554
O2 Y1 O2 116.5(5) 38 78_554
O2 Y1 O2 144.21(15) 22_565 37_455
O2 Y1 O2 73.6(4) . 37_455
O2 Y1 O2 116.5(5) 77 37_455
O2 Y1 O2 69.3(4) 38 37_455
O2 Y1 O2 78.4(5) 78_554 37_455
O2 Y1 O1 90.7(3) 22_565 51_565
O2 Y1 O1 64.5(2) . 51_565
O2 Y1 O1 151.2(3) 77 51_565
O2 Y1 O1 123.6(4) 38 51_565
O2 Y1 O1 83.3(3) 78_554 51_565
O2 Y1 O1 63.9(3) 37_455 51_565
O2 Y1 O1 90.7(3) 22_565 .
O2 Y1 O1 64.5(2) . .
O2 Y1 O1 83.3(3) 77 .
O2 Y1 O1 63.9(3) 38 .
O2 Y1 O1 151.2(3) 78_554 .
O2 Y1 O1 123.6(4) 37_455 .
O1 Y1 O1 121.61(17) 51_565 .
O2 Y1 O1 64.5(2) 22_565 32
O2 Y1 O1 90.7(3) . 32
O2 Y1 O1 123.6(4) 77 32
O2 Y1 O1 151.2(3) 38 32
O2 Y1 O1 63.9(3) 78_554 32
O2 Y1 O1 83.3(3) 37_455 32
O1 Y1 O1 29.6(5) 51_565 32
O1 Y1 O1 130.9(2) . 32
O2 Y1 O1 64.5(2) 22_565 77
O2 Y1 O1 90.7(3) . 77
O2 Y1 O1 63.9(3) 77 77
O2 Y1 O1 83.3(3) 38 77
O2 Y1 O1 123.6(4) 78_554 77
O2 Y1 O1 151.2(3) 37_455 77
O1 Y1 O1 130.9(2) 51_565 77
O1 Y1 O1 29.6(5) . 77
O1 Y1 O1 121.61(17) 32 77
O2 Y1 Y1 39.16(14) 22_565 78_554
O2 Y1 Y1 132.97(19) . 78_554
O2 Y1 Y1 79.5(2) 77 78_554
O2 Y1 Y1 152.0(3) 38 78_554
O2 Y1 Y1 38.3(2) 78_554 78_554
O2 Y1 Y1 106.3(2) 37_455 78_554
O1 Y1 Y1 73.4(3) 51_565 78_554
O1 Y1 Y1 129.7(3) . 78_554
O1 Y1 Y1 44.2(3) 32 78_554
O1 Y1 Y1 102.0(2) 77 78_554
O2 Y1 Y1 39.16(14) 22_565 77
O2 Y1 Y1 132.97(19) . 77
O2 Y1 Y1 38.3(2) 77 77
O2 Y1 Y1 106.3(2) 38 77
O2 Y1 Y1 79.5(2) 78_554 77
O2 Y1 Y1 152.0(3) 37_455 77
O1 Y1 Y1 129.7(3) 51_565 77
O1 Y1 Y1 73.4(3) . 77
O1 Y1 Y1 102.0(2) 32 77
O1 Y1 Y1 44.2(3) 77 77
Y1 Y1 Y1 64.01(7) 78_554 77
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 O1 1.311(18) 77
O1 C1 1.311(18) .
O1 O1 1.311(17) 81
O1 Y1 2.565(12) .
O1 Y1 2.565(12) 81
C1 O1 1.311(18) 9
C1 O1 1.311(18) 77
C1 O1 1.311(18) 73
C1 O1 1.311(18) 5
C1 O1 1.311(18) 81
O2 Y1 2.333(10) .
O2 Y1 2.379(6) 81
O2 Y1 2.379(6) 34
Y1 O2 2.333(10) 22_565
Y1 O2 2.379(6) 77
Y1 O2 2.379(6) 38
Y1 O2 2.379(6) 78_554
Y1 O2 2.379(6) 37_455
Y1 O1 2.565(12) 51_565
Y1 O1 2.565(12) 32
Y1 O1 2.565(12) 77
Y1 Y1 3.678(3) 78_554
Y1 Y1 3.678(3) 77
